General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.83 - 7.85 g/cm³ Show Material materials with Density of 7.83 - 7.85 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa |

20.0 °C | 210 - 212 GPa Show Material materials with Elastic modulus of 210 - 212 GPa | |

100.0 °C | 205 - 207 GPa Show Material materials with Elastic modulus of 205 - 207 GPa | |

200.0 °C | 195 - 199 GPa Show Material materials with Elastic modulus of 195 - 199 GPa | |

300.0 °C | 185 - 192 GPa Show Material materials with Elastic modulus of 185 - 192 GPa | |

400.0 °C | 175 - 184 GPa Show Material materials with Elastic modulus of 175 - 184 GPa | |

500.0 °C | 172.88 - 175 GPa Show Material materials with Elastic modulus of 172.88 - 175 GPa | |

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | |

Elongation | 20.0 °C | 25 - 27 % Show Material materials with Elongation of 25 - 27 % |

Elongation, transverse | 20.0 °C | 23 - 25 % Show Material materials with Elongation, transverse of 23 - 25 % |

Poisson's ratio | 20.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] |

100.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

200.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

300.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

400.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

500.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 81 - 82.19 GPa Show Material materials with Shear modulus of 81 - 82.19 GPa |

100.0 °C | 80.03 GPa Show Material materials with Shear modulus of 80.03 GPa | |

200.0 °C | 76.94 GPa Show Material materials with Shear modulus of 76.94 GPa | |

300.0 °C | 73.69 GPa Show Material materials with Shear modulus of 73.69 GPa | |

400.0 °C | 70.14 GPa Show Material materials with Shear modulus of 70.14 GPa | |

500.0 °C | 66.12 GPa Show Material materials with Shear modulus of 66.12 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 380 - 550 MPa Show Material materials with Tensile strength of 380 - 550 MPa |

Tensile strength, transverse | 20.0 °C | 380 - 550 MPa Show Material materials with Tensile strength, transverse of 380 - 550 MPa |

Yield strength | 20.0 °C | 210 - 235 MPa Show Material materials with Yield strength of 210 - 235 MPa |

Yield strength, transverse | 20.0 °C | 210 - 230 MPa Show Material materials with Yield strength, transverse of 210 - 230 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.11E-5 - 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.11E-5 - 1.25E-5 1/K | ||

200.0 °C | 1.21E-5 - 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 - 1.3E-5 1/K | ||

300.0 °C | 1.29E-5 - 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 - 1.36E-5 1/K | ||

400.0 °C | 1.35E-5 - 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.35E-5 - 1.41E-5 1/K | ||

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | ||

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Max service temperature, long | -25 - 0 °C Show Material materials with Max service temperature, long of -25 - 0 °C | ||

Melting point | 1480 - 1526 °C Show Material materials with Melting point of 1480 - 1526 °C | Typical for Low Carbon Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 460 - 461 J/(kg·K) Show Material materials with Specific heat capacity of 460 - 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | -100.0 °C | 37.6 W/(m·K) Show Material materials with Thermal conductivity of 37.6 W/(m·K) | |

20.0 °C | 42.2 - 52 W/(m·K) Show Material materials with Thermal conductivity of 42.2 - 52 W/(m·K) | ||

100.0 °C | 43.2 - 51 W/(m·K) Show Material materials with Thermal conductivity of 43.2 - 51 W/(m·K) | ||

200.0 °C | 42.9 - 49 W/(m·K) Show Material materials with Thermal conductivity of 42.9 - 49 W/(m·K) | ||

300.0 °C | 41.2 - 46 W/(m·K) Show Material materials with Thermal conductivity of 41.2 - 46 W/(m·K) | ||

400.0 °C | 39.1 W/(m·K) Show Material materials with Thermal conductivity of 39.1 W/(m·K) | ||

500.0 °C | 36.6 W/(m·K) Show Material materials with Thermal conductivity of 36.6 W/(m·K) | ||

600.0 °C | 34.1 W/(m·K) Show Material materials with Thermal conductivity of 34.1 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | -100.0 °C | 12.9 mm²/s Show Material materials with Thermal diffusivity of 12.9 mm²/s | |

20.0 °C | 11.7 mm²/s Show Material materials with Thermal diffusivity of 11.7 mm²/s | ||

100.0 °C | 11.2 mm²/s Show Material materials with Thermal diffusivity of 11.2 mm²/s | ||

200.0 °C | 10.3 mm²/s Show Material materials with Thermal diffusivity of 10.3 mm²/s | ||

300.0 °C | 9.4 mm²/s Show Material materials with Thermal diffusivity of 9.4 mm²/s | ||

400.0 °C | 8.3 mm²/s Show Material materials with Thermal diffusivity of 8.3 mm²/s | ||

500.0 °C | 7.1 mm²/s Show Material materials with Thermal diffusivity of 7.1 mm²/s | ||

600.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | -100.0 °C | 1.82E-7 Ω·m Show Material materials with Electrical resistivity of 1.82E-7 Ω·m |

20.0 °C | 1.2E-7 - 2.47E-7 Ω·m Show Material materials with Electrical resistivity of 1.2E-7 - 2.47E-7 Ω·m | |

100.0 °C | 2.96E-7 Ω·m Show Material materials with Electrical resistivity of 2.96E-7 Ω·m | |

200.0 °C | 3.68E-7 Ω·m Show Material materials with Electrical resistivity of 3.68E-7 Ω·m | |

300.0 °C | 4.55E-7 Ω·m Show Material materials with Electrical resistivity of 4.55E-7 Ω·m | |

400.0 °C | 5.56E-7 Ω·m Show Material materials with Electrical resistivity of 5.56E-7 Ω·m | |

500.0 °C | 6.75E-7 Ω·m Show Material materials with Electrical resistivity of 6.75E-7 Ω·m | |

600.0 °C | 8.13E-7 Ω·m Show Material materials with Electrical resistivity of 8.13E-7 Ω·m | |

Unlock all property charts |

Magnetic

Property | Value | Comment |
---|---|---|

Curie temperature | 770 °C Show Material materials with Curie temperature of 770 °C | Typical for Low Carbon Steel |

Chemical properties

Property | Value |
---|---|

Carbon | 0.17 - 0.24 % Show Material materials with Carbon of 0.17 - 0.24 % |

Manganese | 0.3 - 0.6 % Show Material materials with Manganese of 0.3 - 0.6 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % |

Sulfur | 0.045 % Show Material materials with Sulfur of 0.045 % |